Solvent-controlled elongation and mechanochemical strain in a metal-organic framework
Półrolniczak, Aleksandra; Sobczak, Szymon; Nikolayenko, Varvara; Barbour, Len; Katrusiak, Andrzej; Dalton Transactions  (2021) –; doi:10.1039/D1DT01937F

data_7708720
_publ_section_title
;
 Solvent-controlled elongation and mechanochemical strain in a
 metal-organic framework
;
_journal_name_full               'Dalton Transactions'
_journal_paper_doi               10.1039/D1DT01937F
_journal_year                    2021
_chemical_formula_moiety         'C39 H24 F6 N2 O4 S2 Zn'
_chemical_formula_sum            'C39 H24 F6 N2 O4 S2 Zn'
_chemical_formula_weight         828.09
_chemical_name_common            DMOF
_chemical_name_systematic
1,2-bis(2-ethyl-5-phenyl-3-thienyl)perfluorocyclopentene
_space_group_crystal_system      orthorhombic
_space_group_IT_number           19
_space_group_name_Hall           'P 2ac 2ab'
_space_group_name_H-M_alt        'P 21 21 21'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_audit_creation_date             2019-05-09
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_audit_update_record
;
2019-09-30 deposited with the CCDC.	2021-11-02 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.555(8)
_cell_length_b                   25.56(3)
_cell_length_c                   28.14(7)
_cell_measurement_reflns_used    184
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      9.8160
_cell_measurement_theta_min      3.8420
_cell_volume                     4715(14)
_computing_cell_refinement       'CrysAlisPro 1.171.39.43a (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.39.43a (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.39.43a (Rigaku OD, 2018)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16.2413
_diffrn_detector_type            Eos
_diffrn_measured_fraction_theta_full 0.056
_diffrn_measured_fraction_theta_max 0.671
_diffrn_measurement_details
;
 Data were collected at room temperature and pressure of 1.35(2) GPa
 (1350000 kPa).
 Pressure was determined by monitoring the shift of the ruby R1-fluorescence line.
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Eos'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0108673000
_diffrn_orient_matrix_UB_12      -0.0149342000
_diffrn_orient_matrix_UB_13      -0.0208688000
_diffrn_orient_matrix_UB_21      -0.0616334000
_diffrn_orient_matrix_UB_22      -0.0183047000
_diffrn_orient_matrix_UB_23      0.0125054000
_diffrn_orient_matrix_UB_31      -0.0888572000
_diffrn_orient_matrix_UB_32      0.0146445000
_diffrn_orient_matrix_UB_33      -0.0060323000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.2840
_diffrn_reflns_av_unetI/netI     0.1759
_diffrn_reflns_Laue_measured_fraction_full 0.056
_diffrn_reflns_Laue_measured_fraction_max 0.671
_diffrn_reflns_limit_h_max       3
_diffrn_reflns_limit_h_min       -3
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            3011
_diffrn_reflns_point_group_measured_fraction_full 0.051
_diffrn_reflns_point_group_measured_fraction_max 0.709
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         10.224
_diffrn_reflns_theta_min         4.114
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    0.667
_exptl_absorpt_correction_T_max  0.434
_exptl_absorpt_correction_T_min  0.340
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.39.43a (Rigaku Oxford Diffraction, 2018)
Numerical absorption correction based on gaussian integration over
			a multifaceted crystal model (Absorb Angel (2004) J. Appl. Cryst. 37:486-492)
;
_exptl_crystal_colour            pink
_exptl_crystal_density_diffrn    1.166
_exptl_crystal_description       block
_exptl_crystal_F_000             1680
_exptl_crystal_preparation       'mounted in a diamond-anvil cell '
_exptl_crystal_size_max          0.308
_exptl_crystal_size_mid          0.216
_exptl_crystal_size_min          0.122
_refine_diff_density_max         0.246
_refine_diff_density_min         -0.168
_refine_diff_density_rms         0.053
_refine_ls_abs_structure_details
;
 Flack x determined using 86 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons and Flack (2004), Acta Cryst. A60, s61).
;
_refine_ls_abs_structure_Flack   0.04(15)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.096
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     102
_refine_ls_number_reflns         438
_refine_ls_number_restraints     75
_refine_ls_restrained_S_all      0.998
_refine_ls_R_factor_all          0.1988
_refine_ls_R_factor_gt           0.1498
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
;
 w=1/[\s^2^(Fo^2^)+(0.1271P)^2^+183.4064P]
 where P=(Fo^2^+2Fc^2^)/3
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.3469
_refine_ls_wR_factor_ref         0.3943
_reflns_Friedel_coverage         0.604
_reflns_Friedel_fraction_full    0.045
_reflns_Friedel_fraction_max     0.782
_reflns_number_gt                310
_reflns_number_total             438
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d1dt01937f2.cif
_cod_data_source_block           DMOF_1_35_GPa_Gly
_cod_original_cell_volume        4716(15)
_cod_database_code               7708720